World's largest Science, Technology & Medicine Open Access book publisher


 Kerrie Greer
 3 days ago
 Views:
Transcription
1 PUBLISHED BY World's largest Science, Technology & Medicine Open Access book publisher 3,35+ OPEN ACCESS BOOKS 18,+ INTERNATIONAL AUTHORS AND EDITORS 115+ MILLION DOWNLOADS BOOKS DELIVERED TO 151 COUNTRIES AUTHORS AMONG TOP 1% MOST CITED SCIENTIST 12.2% AUTHORS AND EDITORS FROM TOP 5 UNIVERSITIES Selection of our books indexed in the Book Citation Index in Web of Science Core Collection (BKCI) Chapter from the book Advances in Composite Materials for Medicine and Nanotechnology Downloaded from: Interested in publishing with IntechOpen? Contact us at
2 24 Cavity Enhanced Laser Cooling of Solids Biao Zhong, Youhua Jia and Jianping Yin State Key Laboratory of Precise Spectroscopy, Department of Physics, East China Normal University, Shanghai 262 P. R. China 1. Introduction Since the successful realization of laser cooling of solids in , the optical cooling techniques 25 have made fast development, and laser cooling experiments have obtained some important progress. However, how to improve the absorption of pump laser and enhance the temperature drops so as to realize the practical optical refrigeration, it has become a hot research point in applied physics. As early as 22, the Heeg et. al proposed an extra or intracavity enhancement scheme to improve the laser cooling effect of solids 2, and experimentally demonstrated their intracavity enhancement scheme in 24, and found that there is no large temperature drops due to the experimental parameters were not optimized 3. In 23, Hoyt proposed a multiplepass scheme to enhance the absorption of pump laser and did a series of experimental researches about the multiplepass scheme 4. As expected, a greater temperature drop was obtained. However, due to some limitation in the early work, it is difficulty to cool the sample to the cryogenics temperature, such as low absorption of cooling materials 5, the coating of the sample surfaces 3, the purity of the sample 6, the load from the ambient 1,7, etc. Therefore, people have done much work to improve the record of temperature drop. For example, to avoid the coating absorption deposited on the sample surface, they cut the sample with a Brewster angle along with the cavity axis 8, or improve the purity of cooling material 911, and so on. Mansoor. Seletskiy used the multipass scheme to do some meaningful experiments and obtain a milestone progress, that is, they cool a high pure Yb 3+ doped YLF to cryogenic temperature 12 in this year. To obtain an efficient absorption, another scheme was proposed to insert a Brewstercut sample into a resonant cavity and make the cavity to be resonated with the pump laser, and then the maximum absorption of the pump laser can be achieved 2, Seletskiy demonstrated this scheme in the experiment 13. However, this scheme depends on the power of the pump laser. Fortunately, the intracavity scheme proposed by Heeg can solve this problem in the case of low absorption 2. He also suggested that inserting a cooling sample into the resonant cavity of a laser with a gain (socalled intracavity enhancement scheme) to realize the maximum absorption of the pump laser 2, 14, 19 and carried out it in the experiment 3. Besides of enhancement laser cooling of bulk solids using resonant cavity, we propose another new scheme to optically cool some film materials (i.e., filmier solids) by using a high fineness planar waveguide, which is similar to the cavity enhanced cooling scheme. In our laser cooling scheme, the solid film as a highindex gap waveguide is separated from a prism by a lowindex gap one, and an incident laser beam is resonantly coupled into a
3 618 Advances in Composite Materials for Medicine and Nanotechnology waveguide mode through the gap, by frustrating total internal reflection. This will result in a large enhancement of the pump laser in the solid film and strengthen the effect of laser cooling. In this chapter, some multipass, extra and intracavity enhanced schemes for laser cooling of solids are reviewed and some experimental details of these schemes are discussed. In section 2, multipass laser pump scheme for laser cooling of solids are presented. In section 3, the basic principles of extra and intracavity enhanced resonant absorption for laser cooling of solids are described, and the laser cooling effects between the multipass laser pump and cavityenhancement schemes are compared. In section 4, some experimental results on laser cooling of solids using cavityenhanced technologies and their recent progress are introduced in some detail and reviewed. Some main conclusions and outlook are summarized in the final section. 2. Multipass laser pump scheme for laser cooling of solids In this section, the basic principles of the multipass laser pump scheme to increase absorption for the laser cooling of solids are briefly described, and the corresponding experimental results are introduced in some detail. For the single pass pump geometry, the net power transferred to the sample for the laser radiation can be expressed as 8 hν f hν αb + (1 ηq) αr( ν) αr( ν) ηq total ( ) L Pnet = Pabsη cool = [ Pin (1 e α ν )][ hν ]. (2.1) α ( ν) The negative Pnet corresponds to laser cooling for solids. In Eq.(2.1), Pin is the incident laser power, Pabs is the absorption power of the sample, and ηcool is the cooling efficiency, αb is the background absorption coefficient, which includes both the material s inherent absorption and the frequencyindependent heatgenerated absorption. α r is the resonant absorption coefficient, αtotal( ν ) is the total absorption, which includes a generalized background absorption ( α b ) contributing to heating the sample, resonant absorption ( α r )and an effective absorption due to scattering losses ( α s ), which describe the Fresnel reflections losses from the sample facets 2. L is the physical path length of the laser beam in the sample. Andν andν f are the laser frequency and the mean fluorescent (which represents the mean fluorescent photon energy), respectively. ηq is the external quantum efficiency which represents the fraction of fluorescent emitting from the sample 21 and given by total η W e rad q ηewrad + Wnr η. (2.2) The principle scheme of the multipass pump laser cooling for the cuboid solid sample 4 is shown in Fig 2.1. An incident pump laser beam goes into a solid sample by a hole on the first mirror, and is reflected back at a slightly sloped angle (or along the slightly deviating the incident direction) by the second concave mirror. Taking account of the first bracket term in Eq. 2.1, we can see that if we adopt the multiple pump passes geometry, it will be increased with the number of passes. If the P in is the laser pump power before the first
4 Cavity Enhanced Laser Cooling of Solids 619 mirror, then the absorbed power after multiply passing the sample with α ( ν ) and the length L is expressed as 16 P = P [1 exp( αl)][1 + R exp( αl) + R R exp( 2 αl) + abs in R R exp( 3 αl) + R R exp( 4 αl) + ] n 2 1 in[1 exp( αl)][ ] 1 RR 2 1exp( 2 αl) P αtotal ( ν) L in(1 e ) = P 2 2( RRexp( 2 αl)) 2 2S 1 S N total, (2.3) where N is number of passes, S = R R exp( 2 αl), 2 1 R 1 and R2 are the reflectance of the first and second mirrors, respectively. Fig Multiplepass illustration scheme of cuboid sample laser cooling (figure from ref. [4]) To simplify equation 2.3, we can express the net power transferred to the sample as 3 P = MP e α ν η, (2.4) total ( ) L net in(1 ) cool N where M = (2 2 S ) /(1 S), whenη cool is negative, P net is also negative and represents the cooling power. In recent years, Hoyt et al proposed and demonstrated three multiplepass cooling schemes for solid sample and obtained some good results, which will be introduced as follows: The first is the Brewster sample multipass illustration scheme (see Fig.22). In this scheme, the solid sample is placed between the two mirrors, and the sample is cut as a cuboid geometric shape. It is clear that there are some disadvantages in this scheme, such as the Fresnel reflection losses from the sample facets, or the absorption pump laser contributing to heating due to the antireflection coating on the sample, etc. To avoid these disadvantages above mentioned, Hoyt et al used the Brewstercutting geometry to reduce the Fresnel reflection losses from the sample facets by adjusting the polarization 4 of the incident laser beam.
5 62 Advances in Composite Materials for Medicine and Nanotechnology Fig Multipass illustration scheme of Brewster cut sample (figure from ref. [4]) The second scheme is the mirrored sample multiplepass illumination (see Fig.2.3). In this scheme, the two mirrors are deposited directly on the samples, and the coating is exaggerated. There is a pore on one facet of the sample and the incident laser beam irradiates the sample by this hole, and the orientation of the pump beam deviates slightly the normal of the sample facet so as to multiply reflect the pump light in the sample back and forth. In this case, the absorption of the pump laser can be maximized. Fig Mirrored sample multiplepass scheme (figure from ref. [4]) Fig Total internal reflection scheme of pump beam (figure from ref. [3])
6 Cavity Enhanced Laser Cooling of Solids 621 The last scheme is the total internal reflection one of the pump laser beam, as shown in the Fig In this scheme, the total internal reflection is used to multiply reflect the pump beam in the sample and absorb the pump light as much as possible. For this, one vertex angle of the cubic sample at a diagonal is cut as a small square facet, and the pump beam goes into the sample from this square facet with a small departure, and then the pump laser beam can realize the total internal reflection in the sample, and then the pump beam can be almost absorbed. On the other hand, the above three schemes have individual advantages. From the right term of Eq.2.5, we can see that if we want to maximize the net cooling power P net deposited on the sample, we must maximize the factor M. Therefore in the second scheme when the mirrors are deposited directly on both sides of the sample, the factor M can be effectively maximized 3 because of a potential large number of passes (N). However, this will be detrimental for obtaining a potential large α due to the mirror absorption of the pump laser and resulting in b a heating. This can be avoided in the first scheme because the mirrors are placed at the outsides of the cooling sample, and the effective background absorption will leave the material alone. Unfortunately, M is no longer maxima due to the finite scattering losses (e.g. Fresnel reflections), and there is also the difficulty of the maximizing N, but if adopting the Brewstercut sample, the facet reflections are negligible and the factor M can be increased. Hoyt et al made a cylindrical 1 wt% Tm 3+ : ZBLANP sample with a radius of ~3mm and did some experimental researches for the above scheme 4, 8. In this experiment, the highlyreflecting dielectric mirrors (Cascade optical) are deposited directly on both sides of the sample, and a small entrance aperture for the pump beam is made in one of the mirrors. After coupling the pump laser beam into the sample, unfortunately, the heating effect was observed at all pump wavelengths instead of cooling in the expected wavelength. The experimental results in Fig. 2.5 tell us that the heating magnitude varies with the pump wavelength 22. From Fig. 2.6, it is obvious that there is the water absorption in the mirrors, and this water absorption in the mirrors are contained in the effective total absorption 22 (i.e. added to α =.2 cm 1 ) distributed across the sample length in the mathematics. b Fig Mirrored sample heating with qualitative fit using water absorption (figure from ref. [4])
7 622 Advances in Composite Materials for Medicine and Nanotechnology If using Eq with an additional absorption due to water in the mirrors to fit the experimental data in Fig 2.5, we can obtain the expression of the temperature drop of the sample as follows ΔT [ ( )(1 ) ( ) λ λf καb + αr ν ηq αr νηq ] (2.6) P λ in f Fig Transmission spectrum of the cooling sample with a length of 2μm (figure from ref. [4]) Fig The temperature drops from the room temperature. The bright areas correspond to cooling and the dark to heating (figure from ref. [4])
8 Cavity Enhanced Laser Cooling of Solids 623 The solid line in Fig. 2.5 represents the quantitative fitting. From Fig.2.5 we can see that the change of the sample temperature is dependent on the wavelength of the pump laser. Fig. 2.7 shows the cooling results of the multiplepass pumped cuboid sample in a nonresonant cavity configuration. The pump power is about 3.5W at a wavelength of 1.9 m. We can see from Fig. 2.7 that after the sample is illuminated by the pump laser, the sample temperature starts to be dropped at about 1min, and the sample was cooled to 19 K below the room temperature at the 3min and the sample temperature is no longer changed after ~ 3min. This shows that the net cooling is obvious because the heating from the mirrors that directly deposited on the sample is eliminated, however, the parameters M is not optimized because the pump beam undergoes 4% Fresnel losses at one facet of the sample at each pass 2. To avoid the Fresnel losses, Hoyt et al. used the Brewstercut sample in the nonresonant cavity to improve experimental results, and the corresponding experimental setup and results are shown in Fig. 2.8 and table 2.1. Here the OPO beam is the pump source with a power of 4.35W and 4.5W, which are coupled into the first facet of the two samples, respectively. In the two experiments, the cavity length is about 11cm and the second concave mirrors has a radius of 2 cm, and the change of the sample temperature was measured by recording the phase change in a calibrated MachZehnder interferometer. Fig Laser cooling setup using Brewstercut sample in nonresonant cavity (figure from ref. [4]) Table 2.1. The cooling results of Brewstercut sample (table from ref. [4]) In the table 2.1, τ fit the equation 4 is the fitted time constant, and τ calc is the theoretical time constant from cmρv(1 + χ) τ =, (2.7) 4εσ s 3 s AT s C
9 624 Advances in Composite Materials for Medicine and Nanotechnology where c is the heat capacity per volume, ρ is the sample density, m Vs is the sample volume, Tc is the chamber temperature, As is the sample surface area, andσ is the StefanBoltzmann constant. In addition, the χ in Eq. 2.7 is defined as χ ( ε A / ε A )(1 ε ), (2.8) s s c c c where ε sc, is the emissivity of the sample and chamber. Assuming the unity emissivity for sample and chamber, we can find from table 2.1 thatτ fit are 13.8min and 12min for the two samples, while τ calc are 12min and 7.8min, respectively. So the difference between τ fit and τ calc are approximately 15%, but if presuming the sample emissivity is.9, the difference between τ fit and τ calc is reduced to about 5% in the both cases. Hoyt et al studied the dependences of laser cooling power on the number of passes N for three different multipass schemes: cuboid sample with Fresnel losses in the nonresonant cavity, Brewstercut sample with the same condition as cuboid sample, and a similar sample with the mirrors deposited directly on its facets, and the experimental results are shown in Fig Fig Cooling power modeling for samples with cuboid and Brewster respectively, placed in a nonresonant cavity and a sample with mirrors deposited directly on its facets. (Figure from ref. [4]) In Fig. 2.9, the solid line represents the cuboid sample in nonresonant cavity according to Eq.2.5, and setting the parameters as follows: α b =.2 cm 1, α r =.25 cm 1, η q =.99 and the sample length is.84 cm, the scattering losses α s and Fresnel loss about 4% at each facet per pass are included in the total effective absorptivityα b. The power of pump beam is 1.5W at a wavelength of 1.9 m, and the mean fluorescent wavelength is 1.83 m. The doted line shows the cooling power with the same condition as cuboid sample except without the Fresnel losses due to Brewstercut surface. Taking into account the little loss on the Brewster cut facets, so setting that a loss values is.5% per pass in each facets. The dashed line is also the same calculation other than the mirrors deposited directly on the surface of the sample. Then in the case of α =, the absorption in the mirrors can be added into the background s
10 Cavity Enhanced Laser Cooling of Solids 625 absorption distributed across the sample length 4, so we can set α b =.2 cm 1. The parameters for calculating the cooling power for the mirrors attached directly on the two sides of the samples are arbitrary because it lies on the background absorption in the mirrors 4. So it is the most important for cooling power that reducing the mirror s absorption. If the reflectance of the mirror deposited directly on the sample is 99.95%, then the remaining.5% power was absorbed by the mirrors. As the above discussed, we add this absorption into the background absorption distributed across the sample length. So each mirror has an optical density (OD) of ( α L =.5. ) mirror Fig The relationship between the cooling power and optical density (OD) in the scheme of mirror deposited directly on the samples. (Figure from ref. [4]) Fig. 2.1 describes the relationship between the optical density (OD) and the cooling power for N=5 and 2, respectively. From Fig. 2.1, we can find that the OD must less than the certain value otherwise the cooling power will be become a negative value, which can also be seen from Fig If the value of the OD is larger than.78, there will be no cooling was observed. In 21, D. Seletskiy s group prepared the homeprepared highpurity 5% ytterbiumdoped YLF crystal and cooled it down to the cryogenic temperatures, and the absorption, emission and cooling efficiency spectra of the 5% doped Yb 3+ YLF crystal is shown in Fig In Fig. 2.11, figure (a) represents the absorption and emission spectra, and (b) describes the cooling efficiency. Fitting the experimental cooling efficiency using Eq , we can obtain 4 1 η =.995 andα b = cm. ext 1 ν f ( T) ηc( ν, T) = ηext[ ] 1, (2.9) 1 + α / α( ν, T) ν b whereη ext is the external quantum efficiency, αb is the background absorption, α( ν, T) is the resonant absorption coefficient of the active ion, and ν f is the frequency of the escaped mean luminescent photon, including the reabsorption effect of the emitted fluorescent photon.
11 626 Advances in Composite Materials for Medicine and Nanotechnology Fig Absorption, emission and cooling efficiency spectra of the 5% doped Yb 3+ YLF crystal. The red and blue lines are the absorption and emission spectra respectively for a pump laser with =155nm and polarization along the caxis. The shade of the red line is the cooling tail. Inset: 2 F 5/2 and 2 F 7/2 levels in the crystal position containing seven stark manifolds. Figure b, cooling efficiency curve, the open circles is the experimental data and the line is the mode fitting one. (Figure from ref. [12]) Fig Dependences of the sample cooling temperature on the absorbed power for different pump laser wavelength. The open circles are the experimental data and the solid lines are the mode fitting curves from Eq The blue line indicates the sample used in the experiment can achieve the minimum temperature. (Figure from ref. [23])
12 Cavity Enhanced Laser Cooling of Solids 627 Fig shows the dependences of the cooling temperature of Yb: YLF sample for the pump wavelength at λ = 12nm, 123nm and 13nm, respectively. According to the experimental data in Fig and the StefanBoltzmann law associated with the measured ηabs( ν, T) andη ext, the dependence of the sample cooling temperature on the absorbed power can be modeled 23 as η ν T p ν T = κ T T, (2.1) 4 4 c(, ) abs(, ) ( C ) where Tc is the chamber temperature, and κ is the radiation load constant depending on the geometry and joint thermal emissivities of chamber and sample. In Fig. 2.12, the red, green and blue lines represent the cases of the pump laser wavelength of 13nm, 123nm and 12nm, respectively. The above arrow indicates the previous cooling record in ytterbiumdoped ZBLAN glass, the middle arrow shows the standard thermoelectric coolers (TEC) and the below arrow indicates NISTdefined cryogenic temperature. In this experiment at the maximum available absorbed power of 3.5W at 123nm, the sample is cooled to 155K ± 1K absolute temperature, and the heating is lifted up to 9mW. 3. Resonant cavityenhancement schemes for laser cooling of solids In this section, we review the basic principles and theoretical researches of laser cooling of solid in resonant extra or intracavity, and compare the laser cooling results in the above schemes. Furthermore, we compare the cavityenhancement schemes with the multipass enhancement absorption one. 3.1 Extracavity enhancements for laser cooling of solids Fig. 3.1 shows the scheme of the extracavity enhancement for laser cooling of solids. As shown in Fig. 3.1, the two mirrors with a reflectivity R 1 and R 2 are composed of a resonant extracavity, and the cooling medium with an absorption coefficient α is placed between the mirrors. According to the Beer Law, the loss of the pump beam is proportional to e α d in each pass, and in the same time the other losses including the reflection on the surface of sample and its scattering is defined as x, the pump laser with an intensity of I is coupled into the cavity, and pump/illuminate the sample with a length of L and a lower absorption. The pump beam is reflected on the two cavity mirrors back and forth. If the cavity is resonant with the pump laser, consequently, the beam intensity in the cavity will be resonantly enhanced, and the absorption of cooling sample will be also enhanced. Fig The principle scheme of extracavity enhancement for laser cooling of solids (Figure from ref. [16])
13 628 Advances in Composite Materials for Medicine and Nanotechnology Here we assume that the amplitude of the pump laser is E in the cavity and the corresponding intensity is I, while the amplitude of the incident laser beam before the first mirror R 1 is E and the corresponding intensity is I, and then the amplitude of the laser after each time reflection from R 1 and R 2 are given by E (1 R ) = E, (3.1) E = 1 E exp( 2 ) rr 1 2 ik L, (3.2) E = 2 E exp( 2 ) 1rr 1 2 ik L, (3.3) E exp( 2 ) n = En 1rr 1 2 ik L, (3.4) where r 1,2 are the amplitudes of the reflectivity of the first and second mirrors respectively, and then the total amplitude of the pump beam forward to the right can be expressed as and the corresponding intensity is where δ = 2kL E Ea = E rr ik n L =, (3.5) 1 rr exp( ik 2 L) 2( n 1) ( 1 2) exp[ 2( 1) ] n= I I I = E E = =, (3.6) (1 )(1 ) 1 ( ) 2 cosδ a a a iδ iδ 2 rre 1 2 rre rr 1 2 rr 1 2. When the laser is resonant with the cavity, we have I cosδ = 1, I = a ( rr ) 2rr. (3.7) Assuming the axis of optical cavity is the x axis, the total amplitude of pump laser in the cavity is given by E= ( E e + E e ) e = 2E jsinkxe, (3.8) jkx jkx jwt jwt a a' a and the corresponding intensity of the pump beam is Then the mean intensity of the pump beam can be written as 16 I = E E = I (1 cos2 kx). (3.9) αl a I I = 1 + l [ rr(1 x) e ] α 2 rr(1 x) e. (3.1) In final, the mean enhancement factor is defined as a ratio of the mean intensity of the pump beam in the cavity to the initial intensity of the incident laser beam and given by 16 E _ 2 pcircl I (1 r1 ) cav αl 2 αl Pin I 1 [ rr 1 2(1 x) e ] 2 rr 1 2(1 x) e = = = +. (3.11)
14 Cavity Enhanced Laser Cooling of Solids 629 We take the ZBLAN for an example and set x=.5, l=3mm, and α =.9cm 1, and study the dependence of the enhancement factor E cav of the pump laser in the cavity on both the amplitude r 1 of the reflectivity of the first mirror R 1, and the sample length, and the results are shown in Fig.3.2. Fig (a) The relationship between the enhancement factor E of the pump laser in the cavity and the amplitude of the reflectivity of the first mirror. (b) The relationship between the enhancement factor E cav and the sample length L. (Figure from ref. [16]) In Fig. 3.2 (a), the curve A is the case of the sample surface with an AR coating, which can be used to reduce the losses of reflection on the sample surfaces so as to enhance the intensity of the pump beam in the cavity. The curve B is the case of the sample s surface without an AR coating. It can be seen from the curves A and B that when the reflection loss from the sample surfaces is reduced from the.4 to the.1, the enhancement factor of the pump laser in the cavity is enhanced from the 15 to 28. From Fig. 3.2(b), we can see that with the increasing of the sample length, the enhancement factor will be reduced. This is because the absorption of sample will follow the Beer Law. This shows that by reducing the sample length, one can obtain higher enhancement factor of the pump beam in the cavity, but it also reduce the cooling power. So it is must be taken into account an optimal sample length and a cooling power as high as possible. cav
15 63 Advances in Composite Materials for Medicine and Nanotechnology Then we use the two energy level system to analyze the Yb 3+ level transition between 2F 7/2 2 F 5/2, and obtain an expression of the cooling power in the Extracavity enhancement scheme 24 as follows where αeff P cool NσabsLαeff Is( λ 1) λf * =, (3.12) σ αeff Is 1 + se + σ P abs is the effective irradiation area of the sample, P is the power of pump laser, and Is is the characteristic wavelengthdependent saturation intensity 19, which is defined as I hcγ rad s =, (3.13) λσ abs where σ abs and σ se are the absorption and stimulated emission crosssections respectively, λ is the wavelength of the pump laser, and λf * is the effective mean fluorescent wavelength 7, which can be defined as λ 1 κ ( ) 1 F * =. (3.12) λf hcγrad According to Eq 3.12, we study the dynamic process of the cooling temperature for different pump power, and the results are shown in Fig.3.3. In our calculation, the used parameters come from Ref. [7]. Fig Temperature drop with different pump laser power (Figure from ref. [16]) From Fig.3.3, we can find that with the increase of the pump power from.22w to 2.2W, the temperature of the cooling sample will be reduced from 294.6K to 28.5K. This shows that the extracavity enhanced laser cooling for solid is also very effective. In 26, D. Seletskiy et al proposed another method to describe the extracavity resonant enhancement for optical refrigerator. They assumed that the reflectivity R 2 of the second mirror of the cavity is approximately equal to 1, the absorption coefficient A of the cavity is defined as 13
16 Cavity Enhanced Laser Cooling of Solids 631 A= 1 ( T + R), (3.13) 1 Δ or A =, (3.14) F sin δ where αl 2 ( Ric e ) Δ=, (3.15) αl 2 (1 e R ) ic αl 4e Ric F = αl (1 e R ) ic 2, (3.16) and Ric is the input coupling reflectivity and δ = kl, k is the wave vector inside the absorbing material here assuming that the material fills up the whole cavity, and l is the length of cooling material, and α is the absorption coefficient. From Eq. 3.14, it is clear that A can be 2 l achieve to be unity when Δ and sinδ are set to be zero, i.e., when Ric = e α and δ = mπ. From the above two methods, we find that when the reflectivity R 1 of the incouple mirror is about 95% in the case of setting the same sample absorption, the intensity of the pump beam in the cavity and the absorption of the pump laser can achieve the maximum value. Similar to the extracavity resonant enhancement laser cooling scheme for solids, we proposed a resonant waveguide structure (see Fig.3.4) to effectively cool solid sample, which will enhance the intensity of an evanescent wave by more than two orders of magnitude in the doped Yb 3+ YAG film with a refractive index n 3. The waveguide structure for this scheme is consisted of a prism and two waveguides, which form three layer films with different refraction index n 1, n 2 and n 3 from the bottom to up, here n 2 < n 1 < n 3. The enhancement principle of this resonant waveguide scheme is similar to a FabryPerot cavity with a high finenss 25. On the doped Yb 3+ YAG filmvacuum interface, the light is totally reflected, corresponds to the second mirror of the cavity with a reflection coefficient of 1.. We thus have a FabryPerot cavity with a high fineness: for given values of incident light parameters (e.g. the wavelength), the light field amplitude inside the waveguide will experience a strong resonant enhancement. Fig Scheme of resonant waveguide enhancement for laser cooling of solids
17 632 Advances in Composite Materials for Medicine and Nanotechnology We calculate the enhancement factor of the pump laser in the resonant waveguide structure for the different thickness of doped Yb 3+ YAG film, and the results are shown in Fig.3.5. Enhancement of the field of laser thickness of the Ybdoped YAG film(nm) Fig Dependence of enhancement factor on the thickness of Ybdoped YAG film It is clear from Fig.3.5 that with the increase of the thickness of Ybdoped YAG film, the enhancement factor of the intensity inside Ybdoped YAG film will be greatly increased. In particular, when the thickness of Ybdoped YAG film is increased from 1nm to 16nm, the enhancement factor will be increased from about 2 to 16 times. This shows that our proposed resonant waveguide enhancement scheme can be used to efficiently cool the solid film material. 3.2 Intra cavity enhancements for laser cooling of solids The extracavity resonant enhancement technology is useful to laser cooling of solids due to the greatlyincreased pump laser intensity. However, because the partial transparence of incouple mirror M 1 ( R 1 < 1 ) confines the pump power coupled into the cavity (that is, there is a coupling loss from M 1 ), the enhancement of pumpbeam intensity and the cooling effect of the sample is limited. However, if placing a cooling sample into a resonant cavity of with a gain, we can obtain a greater pumplaser power for laser cooling of solids. This is socalled the intracavity cooling scheme, which is shown in Fig In this scheme, the cooled sample is inserted in the resonant cavity of laser with a gain, and the two mirrors (M 1 and M 2 ) with a reflectivity R 1 and R 2 are the two resonantcavity mirrors of laser with a gain coefficient g. In this case, the two main losses, the absorption loss of sample and the reflection loss of sample surfaces, are added into the original loss δ of the used laser, which forms a total loss δ for the laser. As long as g δ, the used laser can be still satisfied its resonant condition and form a stable laser oscillation. It is clear that the laser intensity in such a laser cavity is far higher than one in a conventional laser because the reflectivity R (= R 1 =R 2 ) of the mirrors in our proposed intracavity cooling scheme can be higher than one R 2 of the output mirror M 2 in a conventional laser. So the intensity of the pump laser in intra  cavity resonant enhancement scheme will be greatly amplified, and an efficient laser cooling for solids will be obtained.
18 Cavity Enhanced Laser Cooling of Solids 633 Fig Intracavity cooling scheme for solids (figure from ref. [14]) It is well known that the output power of a conventional laser system is given by 26 P 1 2g out = s 2 AI T T + δ ( 1), (3.17) where Is is the saturation parameter of laser system, A is the average effective cross section, g is the gain coefficient of laser, δ s is the loss on the surface of sample, δ is the original loss in laser cavity. When the cooling sample is placed in a resonant cavity of laser, the circular power in the cavity is given by 26 P circ = 1 2g AI 2 2 s( 1) T + δ + δs + αd and then the enhancement factor can be expressed as 14, (3.18) 2g 1 Pcirc T + δ + δs + 2αd M = =. (3.19) P 2g out T( 1) T + δ In the low gain case, assuming g =.84, δ =.76, δ =.4 S, and the sample length is 1 d=3cm and α =.9cm, for Yb 3+ doped material. When d=2mm, 3mm, 4mm, according to Eq. 3.19, we study the dependence of the enhancement factor M on the transmittance T of the mirror M 2, and the results are shown in Fig From Fig.3.7, we can see that with increasing of the sample length, the enhancement factor will be reduced because the longer the sample length is, the more the sample absorption of the pump laser is according to Beer Law. However, for a given sample length, the enhancement of the pump beam intensity will be reduced with the increase of the transmissivity T of the output mirror M 2 due to the increase of the output loss from the mirror M 2. The cooling power of the perfect sample placed in the intracavity can be described as 1 f Pcool Pabs P λ = η = λ abs, (3.2) λ
19 634 Advances in Composite Materials for Medicine and Nanotechnology Fig Enhancement factor as a function of transmittance T of the mirror M 2 for different sample length (Figure from ref. [14]) where Pabs is the absorption power of the sample, η is the quantum efficiency that will be slightly reduced during the temperature drop of the sample, simultaneously the mean fluorescent wavelength will be red shift 26, and we have d P = P ( e α 1). (3.21) abs circ Substituting Eq.3.21 into Eq.3.2, and making the assuming that αd is small, Eq can be approximately as 14 P abs 1 2g = αdai 2 2 s( 1) T + δ + δs + αd. (3.22) From Eq.3.22, it is obvious that for the some sample the absorption power of the sample depends on both the sample length and the transmissivity of the output mirror M 2. It is clear in physics that the longer the sample length is, the more the absorption power of the sample is, and then the increasing cavity loss will result in the reduction of the laser oscillating intensity in the cavity. So there must be the optimal length, which can lead to the maximum P abs. dp ( ) By solving the steadystate solution of Eq.(3.22), that is, by solving abs =, we can obtain d( αd) the relationship between the optimal sample length d opt output mirror as follows 14 and the transmissivity T of the 1 αdopt = 2 g( T + δ + δs ) ( T + δ + δs ) 2, (3.23) and the corresponding maximum absorption power is 14 1 P AI g T δ δ 4 2 abs,max = s( S ). (3.24)
20 Cavity Enhanced Laser Cooling of Solids 635 Fig. 3.8 shows the dependence of the optimal sample length on the transmittance T of the output cavity mirror M 2. Fig Optimal sample length as a function of transmittance T of the output mirror M 2 (Figure from ref. [14]) It is clear from Fig.3.8 that the optional sample length will be nearly linearly reduced with increasing the transmittance T of the output mirror M 2. In particular, the sample length does not exceed 2mm in order to obtain a higher enhancement factor and better cooling effect. 3.3 Comparison between multipasses pump and cavityenhancement schemes The enhancement of three schemes, multipasses, extracavity and intracavity, are analyzed in the section 2, subsection 3.1 and 3.2 respectively, and these schemes have their different advantages. In this section, we will compare make the comparison between the multipass pump scheme and two cavityenhancement ones, and hope that one can learn some guiding sense. Firstly, we compare the multipasses pump scheme with the extracavity enhancement one. According to Eq. 2.3, when the reflection times N of the pump beam approach an infinite value, we can obtain the maximum absorption power as follows 14 2 P = P [1 exp( αl)][ ] = 9.7 P [1 exp( αl)], (3.25) abs in 1 RR 2 1exp( 2 αl) in where assuming R 2 = R 1 =99.9%. However, in the extracavity enhancement scheme, the absorption power can be described as Ρ = P [1 exp( αl)], (3.26) abs circ where P circ = E cav P in, according to Eq.3.26 and setting the same parameters, we can obtain Pcirc = 13.8Pin. It is clear that the enhancement factor in the extracavity resonant (absorption) scheme is larger than that in the multipasses one. By comparing the temperature drop in the above two schemes, one can easily observe the advantages of the cavityenhancement. The temperature drop of the cooling sample can be given by 6
21 636 Advances in Composite Materials for Medicine and Nanotechnology and 2 Cmρπ m D d( TS Tr) = Pload ( TS ) Pcool ( TS ), (3.27) 4 dt Bν ( T) Pload = A επ ν Δ Tdν = 4 πdεσbtr Δ T = πdεσb ( Tr TS ), (3.28) T wgere S is the cross section of the sample, Pload is the radiative and conductive load, Cm is the specific heat, ρ m is the mass density, T S and T r are the sample and room temperatures, respectively. Fig. 3.9 is the results of the temperature drop of the multipasses pump and extracavity enhancement schemes. Fig the temperature drop comparison between the multipass pump and the extracavity enhancement schemes (Figure from ref. [14]) From Fig. 3.9, we can find that under the same parameters, the limit of temperature drop in the multipass pump scheme is smaller than that in the extracavity enhancement one. That is, the cooling effect of the extracavity enhancement scheme is better than one of the multipass pump one. Usually, in the resonant extracavity enhancement scheme, the absorption power of the sample for the pump can be easily calculated by the multiabsorption. However, in the intracavity enhancement scheme, before calculating the absorption power of of the sample for the pump laser, we first have to calculate the laser power in the cavity. In order to compare the intracavity enhancement scheme with the extracavity one, we define the input power of the extracavity by the gainsaturation formula 26 P 1 g in = s 2 AI T T + δ ( 1), (3.29) where T is the transmittance of the couple mirror M 1, Is is the system saturation parameter, and g is the gain of laser gain medium. Once the pump beam passes the sample, the absorption power of the sample for the pump laser can be expressed as2, 19 1 g = = ext αl P (1 e )(1 R ) (1 )(1 ) ( 1) abs, s s Pin Ts Rs AIsT 2 T + δ. (3.3)
22 Cavity Enhanced Laser Cooling of Solids 637 After the pump beam Nth passes through the sample, the total effective absorption power of the sample is given by 2, 19 N n 1 ext 1 (1 αl g )(1 ) ( P = e Rs AIsT 1) ( θts ) abs 2 T δ n= 1 1 g 1 ( θts ) = e R AI T 2 T + 1 θ T αl (1 )(1 s) s ( 1) δ + (3.31) By optimizing the output coupler (d P in /dt=) for maximum P in, we have S N. (3.32) ext So the maximum of P can be obtained by abs T = g δ δ. (3.33) opt 2, ( θt ) P e R AI T g N ext αl 2 S = (1 )(1 ) (, ) abs opt s s δ 2 1 θts. (3.34) For the sake of convenience, Eq and 3.21 are written in dimensionless, respectively 2, 19 1 ( θt ) N ext αl 2 S = (1 )(1 )(, ) abs opt s δ 1 θts P e R g, (3.35) 2 and P g abs = α d ( 1). (3.36) T + δ + δ + 2α d Under the low gain conditions, and according to Ref [3], we have g =.89 and δ =.78, which were measured for a practical cw pumped dye laser system by placing an acoustooptic modulator (EOM) inside the cavity. We used δ S =.4, R s =.1 to calculate and analyze the dependence of the absorption power of the sample on the optical density for the different numbers N of passes, and the results are shown in Fig S Fig Absorption power of the sample in the external cavity scheme with different numbers N of passes and the intracavity scheme as a function of the optical density. (Figure from ref. [19])
23 638 Advances in Composite Materials for Medicine and Nanotechnology From Fig.3.1, we can find that for the low optical density, specially as α d <.8, the absorption power in the intracavity scheme is far high than that in the extracavity one. However, when α d >.1, because the losses from the sample approach the laser threshold, the absorption power will be sharply decreased. So in the region of the large optical density, the absorption power in the extracavity scheme is far higher than one in the intracavity one. As shown in Fig. 3.1, if we increase the pass number N of the pump beam, the absorption power in the extracavity scheme will increase to even exceed one in the intracavity scheme. 4. Experiment studies on laser cooling of solids using cavityenhanced technologies In the above section, we discuss and compare the enhancement effect of laser cooling of solids in the multipass pump, intracavity and resonant extracavity schemes in some detail. In this section, we will review experimental researches on laser cooling of solids using the above cavityenhanced schemes and its recent progress. As early as 23 years, Hoyt et al. at University of New Mexico 4 and LANL group did detailed experimental research on laser cooling of solids 8 by using the multipass scheme after proposing how to improve the absorption power of the pump laser. At the same year, Heeg proposed the two methods using the intracavity and extracavity scheme to enhance the absorption power for laser cooling of solids and comparing laser cooling efficiencies between the intracavity and extracavity schemes. Afterwards, Heeg group demonstrates the intracavity solidstate laser cooling of solids in experiment 3. Seletskiy s group and LANL did a series of experimental researches on the cavityenhanced resonant absorption for laser cooling of solids and obtained some important progress. More recently, they have successfully completed a milestone work and realized laser cooling of dopedyb +3 YLF crystal materials with a cryogenic temperature. 4.1 Cooling of Yb: ZBLAN using intracavity enhanced absorption When a diode laser is used to pump a solid laser, the laser radiation will be oscillated in an optical resonant cavity, at the same time the intensity of laser in the cavity will be amplified due to the simulation emission of laser gain medium. After the intensity of laser in the optical resonant cavity exceeds its threshold, the laser will be output from the cavity 26. If inserting a solid sample with a low loss into the optical cavity, but the excited wavelength can be sustained to be oscillated in the cavity, and then the intracavity enhanced laser will increase the resonant absorption of the sample, which will result in an efficient laser cooling for solids in the laser cavity. As discussed in section 3.1, the almost materials used to form optical refrigeration has a low optical density (i.e., a low absorption), so one can use this intracavity enhanced scheme to realize laser cooling of solids. By choosing some optimal parameters, the intracavity enhancement scheme will become an efficient laser cooling method. In 24, Heeg group demonstrated the intracavity solidstate laser cooling scheme for solids experimentally 3 and the corresponding experiment setup is shown Fig In their experiment, the Yb 3+ KY (WO 4 ) 2 (KYW) gain medium (1% doped, 1mm length, antireflection coated) was pumped along its b axis in the longitudinal direction by either one or two counterpropagating diode laser ( 1 1μm ) at 981.2nm. The diode laser was focused into the gain medium, which was
24 Cavity Enhanced Laser Cooling of Solids 639 placed at the confocal center of a Z cavity, by using two concave mirrors with a high reflectivity at 1216nm and a high transmission at 981.2nm. About 3W laser power per diode was illuminated on the gain medium due to the reflection losses from the pump optics. A Brewster prism was used to tune the excited wavelength from about 12nm to 14nm. A spatial filter was utilized here to minimize the residual radiation and super fluorescence on the cooling medium. An output coupling mirror with a 2% transmission was used to output a laser beam with the maximum power of up to 8mw at 132nm when the power each diode laser is 1.2W. The intracavity circulating powers was be increased to 18W by using a high reflectivity mirror. Fig Schematic of intracavity enhancement laser cooling of solids. LD is the laser diode, PD is the photodiode, HR is the high reflector, BP is the Brewster tuning system, and SF is the spatial filter. (Figure from ref. [3]) The cooling medium, a 2% doped Yb 3+ : ZBLAN rectangular glass with dimensions 2 2 3mm, is used in this experiment, and the endfaces of the cooling medium is cut as a Brewster s angle in order to reduce the reflection losses of the sample surfaces. In the experiment, the temperature change of the sample is measured by a noncontact fashion according to the fluorescent spectral narrowing with decreased homogeneous broadening at lower temperatures. They measured the temperature drop spectrum of the cooling sample with a 2mm length, and the results are shown in Fig In this experiment, the gain medium was pumped by two diode laser and the pump power in the cavity was up to 125W. After 1 minutes the sample reached the new thermal equilibrium and its temperature dropped to 6 K from the ambient temperature. At the same time, the heat sink s temperature rises by 3K due to absorbing the scatter laser and fluorescent emitted by the sample. This experiment demonstrated the intracavity enhancement for laser cooling of solids. Because the absorption of cooling medium is low and the laser power for the optical refrigerator is not very high, so this approach is a prospect method for future optical refrigerator. The temperature drop of the cooling medium is not large in this experiment
25 64 Advances in Composite Materials for Medicine and Nanotechnology due to not enough pure of the sample and resulting in parasitic heating 27, the thermal radiation from the chamber, the conductive thermal from the supporter, the reapportion fluorescent 28, 29, 3, however, these problems will be improved in the future along with the advance of material fabrication 9, low emissivity coating and so on. Furthermore, introducing the Brewster prism to tune the wavelength is very important for cooling the sample to the cryogenic temperature. This is because with the temperature drop the population in the ground upper multilevels will be decreased, so it must adjust the wavelength to the short wavelength so as to weaken the decreasing absorption of the pump beam, and is able to obtain the cryogenic temperature 11,31. Finally, the intracavity cooling approach has prosperously perspective for the practical optical refrigerator. Fig The temperature change of the sample with a 2mm length and the heat sink as function of time (Figure from ref. [3]) 4.2 Cooling of Yb: ZBLAN using extracavity enhanced resonant absorption The multipass scheme make great successful in laser cooling of solids in Ref [12] and obtain 143K temperature drop from room temperature, but it has own disadvantage. One of the fundamental defects is a hole on the endface of the sample because it will introduce light scattering (parasitic loss) and leak the pump light. Another shortcoming is the mirror deposited on another endface of the sample, which will lead to the parasitic heating. The intracavity scheme has some advantages, such as the higher pump laser intensity in the cavity and an adjustable pump wavelength by the Brewster tuning prism 3, but it has not been adopted usually due to more optical components in the cavity and the complexity of operation. So it goes against to develop a practical optical refrigeration due to these disadvantage of the above two schemes. Fortunately, the extracavity resonant enhancement laser cooling scheme for solids offers a relatively simple and feasible technology for optical refrigeration.
26 Cavity Enhanced Laser Cooling of Solids 641 Fig Schematic experimental setup of the extracavity resonant enhancement laser cooling The schematic experimental setup for extracavity enhancement resonant absorption for laser cooling of solids is shown in Fig The cavity is made up of two mirrors, and the first mirror M 1 is the input coupling mirror with a reflectivity of 95%, which can be adjusted to the proper value so as to obtain the maximum resonant absorption of cooling medium according to the absorption of the cooling material and the loss in the cavity. The reflectivity of the second mirror M 2 is almost equal to unity. In this experiment, the laser wavelength should be resonant with the optical cavity with a length of l so that one can obtain the maximum power in the cavity and the maximum absorption of cooling medium. A small amplitude signal generated by the function generator is used to dither the cavity, and then the intensity of laser is modulated, simultaneously, this signal is also input into LockIn Amplifier as a reference signal. The dithered transmission is monitored by the photodetector and mixed it with the reference signal from the function generator in LockIn Amplifier. Then the error signal demodulated by LockIn Amplifier was feedback to the PZT on the mirror after amplified by the HighVoltage Amplifier. Thus one can keep the laser frequency to be resonant with the frequency of cavity. The temperature of solid sample can be monitored by the thermal camera or Differential luminescence thermometry In 26, D. Seletskiy et al studied the cavity enhanced resonant absorption for laser cooling of Yb 3+ ZBLAN glass in experiment 13. A commercial laser (ELS, VeraDisk Yb: YAG) with the maximum output power of about 45W at 13nm was used. To avoid the laser unstable due to the optical feedback, a Faraday isolator (EOT, Model# 4I13) with > 3dB isolation was used. The MML 2 and MML 1 (MML 1 with f1=5 mm, MML 2 with f2=1mm) coating with antireflection coat for 13nm on their sides was used to enable the laser beam has a proper divergence and a proper transverse mode inside the cavity 26. The input coupler was mounted on the 3axis piezocontrollers (Thorlabs, Part#MDT693) to control the transverse mode of the cavity to match with that of the laser. The reflectivity of the coating on the sample endface serve as high reflection mirror is higher than 99.9%.
27 642 Advances in Composite Materials for Medicine and Nanotechnology Fig The relationship between the cavityenhanced absorption and the inputcoupler reflectivity for two different values ofα l (Figure from ref. [13]) From the extracavity enhancement theory in section 3.1, D. Seletskiy calculated the inputcoupler reflectivity as a function of the sample absorption for different optical density α l, and the results are shown in Fig In the experiment, D. Seletskiy et al demonstrated the absorption enhancement for two different inputcoupler reflectivities, and the results are shown in Fig We can see from the theoretical calculation (see Fig.4.4) and the experimental results (see Fig.4.5) that the experimental data are in good agreement with the theoretical results, which can be further found in Fig In this work, D. Seletskiy et.al did not give the temperature drop of the sample, but just to prove the enhancement of resonant absorption of Yb: ZBLAN glass sample by a factor of 11 compared to the doublepass configuration. This is the great significance meaningful work because it has relatively simple optical arrangement and great enhancement of the absorption for the cooling sample. Fig Experimental demonstration of the absorption enhancement for two different inputcoupler reflectivities R ic = 9% and 94%, respectively (Figure from ref. [13])
28 Cavity Enhanced Laser Cooling of Solids 643 Fig The dependence of the enhancement absorption factor on the reflectivity of Inputcoupler, and the shaded region represents uncertainty in the measured value of α l=.45 ±.5. The enhancement factors γ are plotted in the same scale, which is obtained from the experiments with different reflectivities (9%, 94%, 99%) and show very good agreement with the expected values, calculated from Eq (Figure from ref. [13]) After this work, D. Seletskiy et al did a series of work to improve the extracavity enhancement for laser cooling of solids and made the great achievements, and nearly 2 fold of enhancement of the resonant absorption are obtained. Fig Experimental setup of extracavity resonant enhancement scheme for laser cooling of solids. The thin lines are the optical beam path, and the thicker lines are electronic connections. (Figure from ref. [1]) Fig. 4.7 is the improved experimental setup. In this experiment, the reflectivity of the dielectric mirror is greater than 99.99%, and the sample was supported by 4 quartz 6 m
29 644 Advances in Composite Materials for Medicine and Nanotechnology diameter fiber. The sample was placed in a clamshell, which was placed in the aluminum vacuum chamber with 8 vacuum ports, and the windows were coated by AR coating to increase the transmission of the pump laser. The inside surfaces of clamshell chamber are painted with a preferential lowemissivity Maxorb coating, which is a goldplated copper. The cavity is kept on working resonant with the pump wavelength and is stabilized via an electronic feedback loop. In this experiment, they obtained the absorption efficiency up to 91 ± 2%, and the temperature drop was about 3K, which was measured by a noncontact method, socalled differential luminescence. This measurement method is so sensitive that can resolve a.1k temperature change by resolving the temperature change from the reference spectra. In 28, D. Seletskiy et al studied the cavity resonantenhanced laser cooling of Yb 3+ : YLF crystal and obtained the temperature drop of about 7 degrees from the ambient temperature. In the experiment, the sample was cut with a Brewster angle to reduce the Fresnel loss in the endfaces of the sample, and the cavity is also formed in Brewster geometry for the ppolarized pump light. Fig. 4.8 is the photograph of Brewster geometry cavity. From Fig.4.8, we can see that in order to reduce the loss of cavity, the mirrors should be almost contacted with the sample. Fig Photograph of the Brewster geometry cavity. The left mirror of the image is the input coupler mounted on the 3axis piezo mirror mount. The fiber above the sample is used for collecting luminescence. False color luminescence is visible in the sample, induced by pump light trapped on resonance. (Figure from ref. [17]) Fig. 4.9 shows the experiment results on the temperature drop of the sample for the different input power. Due to the sample so close to the mirror, the fluorescent emitted from the sample will be absorbed by the mirror. Simultaneously, the mirror with a nearly unity emissivity at the thermal wavelengths radiates on the sample and heats it. So the temperature drops of the Yb: YLF crystal is up to 69K from the room temperature. This is the cooling record for crystalline solids, but it not achieves the minimum achievable temperature (MAT). However, under the ideal conditions, the MAT could be achieved to 17 ± 1K [12]. In this year, D. V. Seletskiy investigate the resonant cavityenhanced absorption for optical refrigeration with a lowpower laser and find the 2fold increase over the single path absorption with the low loss medium (Yb 3+ doped ZBLAN glass 23 ) placed in the resonant
30 Cavity Enhanced Laser Cooling of Solids 645 cavity mentioned. Their experiment setup is shown in Fig The 2% Yb 3+ doped ZBLAN glass was placed in the cavity, and one endface of the sample was coated as a high reflectivity of mirror (R>.999), and another face of the sample was deposited a antireflection coating to decrease Fresnel loss on the surface. Fig The top graph shows the temperature dynamicsδt(offset to zero at 298K). The grey closed circles, the red solid line and the blue open circles represent the temperature change of the sample, cavity mirrors and the difference temperature of the chamber and sample, respectively. The bottom graph is the absorption on linear scale in arbitrary units. (Figure from ref. [17]) Fig The arrangement of experimental setup. PD+LA+PID is the proportional integralderivative circuit, PD is the piezo driving circuit, LA is the lockin amplifier, which are used to control the cavity length to keep stabilization. TC is the thermal camera for monitoring the cooling process. (Figure from ref. [23]) To optimize the maximum pump laser coupled into the cavity, the reflectivity of the input l mirror is usually equal to the value of Ric = e α. The input mirror with a reflectivity of R=94% is housed in a piezoactuated mount, allowing for cavity length scanning and stabilization. Moreover, to minimum the heat load adding to the sample, thin quartz fibers used to support the sample, which is placed in a tightly fitted shell with a lowemissivity coating. The cooling process is recorded by the thermal camera. Due to the transmission and losses are minimized by design, so the absorption A can be deduced from A=1R c. In the GiresTournois limit, the pump absorption at resonance can be expressed as 23
31 646 Advances in Composite Materials for Medicine and Nanotechnology αl RI e A = 1 ( ). (4.1) αl 1 e R I Fig (a) Resonant 89% absorption of the cavity plotted on a semilog scale. (b) The experiment data agree with model fitting results, according to Eq (Figure from ref. [23]) Fig (a) shows the relationship between the cavity reflectivity and the cavity length. From Fig.4.11(a), we can find that the maximum absorption reaches to 89 ± 3% when the cavity length are scanned. From Fig (b), it is clear that the resonant cavity enhancement factor is up to 2 fold compare with singletime passing the sample. Fig. 4.1 is the experimental results of cooling process and the temperature drop of the sample. To avoid the saturation of the thermal camera image, the sample was radiated by the pump laser with a 1W power for 4 minute. Fig (a) Top view thermal image of the cavity at resonance. Blue area represents the sample, the green area represents the ambient and light gray structure around the sample is the shell, which is heat by the fluorescence absorption. (b) The red line is the experiment measurement data, and the gray dot line is the fitting one. (Figure from ref. [23]) By fitting the experimental data to Δ Tt ( ) =ΔTf [1 exp( t/ τ )], they obtain the final temperature drop of Tf = 3.2 ±.1K from the ambient. Form the fitting formula, the thermal time constant is τ = 45 min. In the case of small input power, the temperature drop linearly scales to be imperfect efficiencies. The ratio of absorption, stabilization, radiation shielding are 9%, 6%, and 3% respectively. It can be estimated that the final temperature drop 1 is 3.2 [.9.6.3] = 2 K/ W. The difference between the above mentioned final temperature drop per unity power of incident laser (2K/W) and the best cooling performance of 22 K/ W in Yb: ZBLAN glass can be ascribed to the variation of the impurity of the different sample.
32 Cavity Enhanced Laser Cooling of Solids Conclusions and outlook In this chapter, we have reviewed various enhancement means of the pump beam to facilitate laser cooling of solids, and especially discussed the multipass pump, extracavity and intracavity resonant enhancement absorption in some detail from their principles to the experiment technologies. Although the multipass pump scheme has a lower absorption enhancement relative to two other schemes, it has simple operation and less optical elements. Therefore one hope to find some more efficient material for laser cooling or develop some high purity of solids, and first using the multipass pump scheme to do experimental researches on laser cooling of solids, such as using Yb 3+ doped ZBLAN and Yb 3+ doped YLF materials in the experiments. So the multipass scheme can compete with other two cavityenhanced ones in the factual optical refrigerator. The intracavity enhancement scheme can greatly enhance the intensity of the pump laser in the cavity when the lowloss cavity and low absorption of cooling medium is used, however, due to the complication of technology and more optical elements, it will lead to some obstacles for forming a feasible optical refrigerator. In particular, it will be no suitable for some cooling materials with a large absorption. Since the extracavity enhancement scheme is a relatively simple technology and has a large enhancement of resonant absorption, it would be chosen as one of the practical or useful optical refrigerators. The scientists have used the three different schemes mentioned above to investigate laser cooling of solids in experiment and hoped to find a more feasible technology for the future optical refrigeration. By optimizing the experiment parameters, one hope to obtain the maximum temperature drops of laser cooling samples. Furthermore, by probing some new coating materials to shield the thermal radiation more effectively, adjusting the geometry of the sample, and reducing the impurity of the sample, one hope to find some new paths to a practical optical refrigerator. Recently, D. V. Seletskiy utilizing the extracavity resonant enhancement scheme to improve the pump laser absorption by up to 2 folds compared with the single pass pump one. In this year, especially, laser cooling of solids to cryogenic temperatures using the multipass enhancement absorption shows a new dawn to develop a promising optical refrigerator. Since such an alloptical refrigerator has some novel and unique advantages, such as a mini volume, lightly weight, electromagnetic radiation free, nonvibration, nonnoise, and long lifetime, etc, it will become an irreplaceable cryogenics in the fields of military, space technology, integrated optics, microelectronics, remote sensing and telemetering, and so on. 6. Acknowledgments We acknowledge the support from the National Natural Science Foundation of China under Grant No References [1] R. I. Epstein, M. I. Buchwald, B. C. Edwards, T. R. Gosnell. C. E. Mungan, Nature, 1995, Vol. 377(12): [2] B. Heeg, G. Rumbles, A. Khizhnyak, P. A. DeBarber, J. Appl. Phys, 22, Vol. 91(5): [3] B. Heeg, M. D. Stone, A. Khizhnyak, G. Rumbles, G. Mills, P. A. DeBarber, Phys. Rev. A, 24, Vol. 7: 2141(14) [4] Chad. William. Hoyt, The University of New Mexico, PHD May 23
33 648 Advances in Composite Materials for Medicine and Nanotechnology [5] C. W. Hoyt, M. SheikBahae, R. I. Epstein, B. C. Edwards, and J. E. Anderson, Phys. Rev. Lett, 2, Vol. 85 (17): [6] T. R. Gosnell, Opt. Lett. 1999, Vol. 24: [7] X. Luo, M. D. Eisaman, and T. R. Gosnell, Opt. Lett. 1998, Vol. 23: [8] C. W. Hoyt, M. P. Hasselbeck, M. SheikBahae, J. Opt. Soc. Am. B, 23, Vol. 2, (5) [9] M. P. Hehlen, R. I. Epstein, SPIE, 27, Vol. 6461, 64613(16) [1] W. M. Pattersona, M. P. Hehlenb, M. SheikBahaea, R. I. Epstein, SPIE, Vol. 7228: 7228C(11) [11] R. I. Epstein, M. SheikBahae, Optical Refrigeration science and applications of laser cooling of solids, 21 [12] D. V. Seletskiy, S. D. Melgaard, S. Bigotta, A. D. Lieto, M. Tonelli, M. SheikBahae, Nature Photonics, 21, 17: [13] D. Seletskiy, M. P. Hasselbeck, M. SheikBahae, J. Thiede, R. I. Epstein, SPIE 26, Vol 613: 613p(18) [14] Y. H. Jia, B. Zhong, J. P. Yin, Chin. Phys. Lett, 28, Vol. 25(1): [15] D. Seletskiy, M. P. Hasselbeck, M. SheikBahae, R. I. Epstein, SPIE, 27, Vol. 6461: 64614(18) [16] Y. H. Jia, B. Zhong, J. P. Yin, Chin. Opt. Lett, 28, Vol. 6(11): [17] D. Seletskiy, M. P. Hasselbeck, M. SheikBahae, R. I. Epstein, S. Bigottac, M. Tonelli. SPIE 28, Vol. 697: 697B(19) [18] D. V. Seletskiy, S. D. Melgaard, M. P. Hasselbeck, M. SheikBahae, R. I. Epstein, S. Bigottac, M. Tonelli, SPIE, 29, Vol. 7228: 7228F(14) [19] Y. H. Jia, B. Zhong, J. P. Yin, Chin. Phys. Lett, 21, Vol 7: 7321(14) [2] M. Born, E. Wolf, Principled of Optics (Seventh Edition) [21] A. Rayner, N. R. Heckenberg, H. Rubiszteindunlop, J. Opt. Soc. Am. B, 23, Vol. 2(5): [22] L. H. Kou, D. Labrie, P. Chylek, Applied. Optics 1993, Vol. 32(19): [23] D. V. Seletskiy, M. P. Hasselbeck, M. SheikBahae, App. Phy. Lett, 21, Vol. 96: 18116(14) [24] C. E. Mungan, M. I. Buchwald, B. C. Edwards, R. I. Epstein and T. R. Gosnell, Phys. Rev. Lett, 1997, Vol. 78(6), [25] G. Labeyrie, A. Landragin, J. V. Zanthier, R. Kaiser, N. Vansteenkiste, C. Westbrook. A. Aspect, Quantum. Semiclass. Opt, 1996, Vol. 8: [26] A. E. Siegman, Lasers, University Science Books, Sausalito, 1986 [27] J. C. Fajardo,G. H. Sigel Jr, B. C. Edwards, R. I. Epstein, T. R. Gosnell, C. E. Mungan, J. NonCryst. Solids, 1997, Vol. 213&214: 951 [28] B. Heeg, G. Rumbles, J. Appl. Phys. 23, Vol. 93(4): [29] B. Heeg, P. A. DeBarber, and Garry Rumbles, Applied. Optics, 25, Vol. 44(15): [3] X. F. Wang, S. L. Chang, J. K. Yang, M. Zhou, D. X. Cao, J. C. Tan, Applied. Optics, 27, Vol. 46(35): [31] M. SheikBahae, R. I. Epstein, Nature. Photonics, 27, Vol. 1: [32] B. Imangholi, M. P. Hasselbeck, D. A. Bender, C. G. Wang, M. SheikBahae, R. I. Epstein, S. Kurtz, SPIE, 26, Vol. 6115: 61151C(16) [33] W. Patterson, E. Soto, M. Fleharty, M. SheikBahae, SPIE, 27, Vol. 6461: 6461B(16) [34] D. V. Seletskiy, M. P. Hasselbeck, M. SheikBahae, R. I. Epstein, SPIE, 29, Vol. 7228: 7228K(15) [35] W. M. Patterson, D. V. Seletskiy, M. SheikBahae, R. I. Epstein, M. P. Hehlen, 21, J. Opt. Soc. Am. B, Vol. 27 (3):
34 Advances in Composite Materials for Medicine and Nanotechnology Edited by Dr. Brahim Attaf ISBN Hard cover, 648 pages Publisher InTech Published online 1, April, 211 Published in print edition April, 211 Due to their good mechanical characteristics in terms of stiffness and strength coupled with masssaving advantage and other attractive physicochemical properties, composite materials are successfully used in medicine and nanotechnology fields. To this end, the chapters composing the book have been divided into the following sections: medicine, dental and pharmaceutical applications; nanocomposites for energy efficiency; characterization and fabrication, all of which provide an invaluable overview of this fascinating subject area. The book presents, in addition, some studies carried out in orthopedic and stomatological applications and others aiming to design and produce new devices using the latest advances in nanotechnology. This wide variety of theoretical, numerical and experimental results can help specialists involved in these disciplines to enhance competitiveness and innovation. How to reference In order to correctly reference this scholarly work, feel free to copy and paste the following: Biao Zhong, Youhua Jia and Jianping Yin (211). Cavity Enhanced Laser Cooling of Solids, Advances in Composite Materials for Medicine and Nanotechnology, Dr. Brahim Attaf (Ed.), ISBN: , InTech, Available from: InTech Europe University Campus STeP Ri Slavka Krautzeka 83/A 51 Rijeka, Croatia Phone: +385 (51) Fax: +385 (51) InTech China Unit 45, Office Block, Hotel Equatorial Shanghai No.65, Yan An Road (West), Shanghai, 24, China Phone: Fax: